Ge/Si(001) heterostructures with dense arrays of Ge quantum dots: morphology, defects, photo-emf spectra and terahertz conductivity
© Yuryev et al.; licensee Springer. 2012
Received: 20 May 2012
Accepted: 16 June 2012
Published: 23 July 2012
Issues of Ge hut cluster array formation and growth at low temperatures on the Ge/Si(001) wetting layer are discussed on the basis of explorations performed by high resolution STM and in-situ RHEED. Dynamics of the RHEED patterns in the process of Ge hut array formation is investigated at low and high temperatures of Ge deposition. Different dynamics of RHEED patterns during the deposition of Ge atoms in different growth modes is observed, which reflects the difference in adatom mobility and their ‘condensation’ fluxes from Ge 2D gas on the surface for different modes, which in turn control the nucleation rates and densities of Ge clusters. Data of HRTEM studies of multilayer Ge/Si heterostructures are presented with the focus on low-temperature formation of perfect films.
Heteroepitaxial Si p–i–n-diodes with multilayer stacks of Ge/Si(001) quantum dot dense arrays built in intrinsic domains have been investigated and found to exhibit the photo-emf in a wide spectral range from 0.8 to 5 μ m. An effect of wide-band irradiation by infrared light on the photo-emf spectra has been observed. Photo-emf in different spectral ranges has been found to be differently affected by the wide-band irradiation. A significant increase in photo-emf is observed in the fundamental absorption range under the wide-band irradiation. The observed phenomena are explained in terms of positive and neutral charge states of the quantum dot layers and the Coulomb potential of the quantum dot ensemble. A new design of quantum dot infrared photodetectors is proposed.
By using a coherent source spectrometer, first measurements of terahertz dynamical conductivity (absorptivity) spectra of Ge/Si(001) heterostructures were performed at frequencies ranged from 0.3 to 1.2 THz in the temperature interval from 300 to 5 K. The effective dynamical conductivity of the heterostructures with Ge quantum dots has been discovered to be significantly higher than that of the structure with the same amount of bulk germanium (not organized in an array of quantum dots). The excess conductivity is not observed in the structures with the Ge coverage less than 8 Å. When a Ge/Si(001) sample is cooled down the conductivity of the heterostructure decreases.
Artificial low-dimensional nano-sized objects, like quantum dots, quantum wires and quantum wells, as well as structures based on them, are promising systems for improvement of existing devices and for development of principally new devices for opto-, micro- and nano-electronics. Besides, the investigation of physical properties of such structures is also of fundamental importance. In both regards, amazing perspectives are provided when playing around with quantum dots that can be considered as artificial atoms with a controlled number of charge carriers that have a discrete energy spectrum[1, 2]. Arrays of a large number of quantum dots including multilayer heterostructures make it possible to create artificial “solids” whose properties can be controllably changed by varying the characteristics of constituent elements (“atoms”) and/or the environment (semiconductor matrix). The rich set of exciting physical properties in this kind of systems originates from single-particle and collective interactions that depend on the number and mobility of carriers in quantum dots, Coulomb interaction between the carriers inside a quantum dot and in neighbouring quantum dots, charge coupling between neighbouring quantum dots, polaron and exciton effects, etc. Since characteristic energy scales of these interactions (distance between energy levels, Coulomb interaction between charges in quantum dots, one- and multiparticle exciton and polaron effects, plasmon excitations, etc.) are of order of several meV[3–5], an appropriate experimental tool for their study is provided by optical spectroscopy in the far-infrared and terahertz bands.
To get access to the effects, one has to extend the operation range of the spectrometers to the corresponding frequency domain that is to the terahertz frequency band. Because of inaccessibility of this band, and especially of its lowest frequency part, below 1 THz (that is cm−1), for standard infrared Fourier-transform spectrometers, correspondent data is presently missing in the literature. In this paper, we present the results of the first detailed measurements of the absolute dynamical (AC) conductivity of multilayer Ge/Si heterostructures with Ge quantum dots, at terahertz and sub-terahertz frequencies and in the temperature range from 5 to 300 K.
In addition, for at least two tens of years, multilayer Ge/Si heterostructures with quantum dots have been candidates to the role of photosensitive elements of monolithic IR arrays promising to replace and excel platinum silicide in this important brunch of the sensor technology[6–8]. Unfortunately, to date achievements in this field have been less than modest.
We believe that this state of affairs may be improved by rigorous investigation of formation, defects and other aspects of materials science of such structures, especially those which may affect device performance and reliability, focusing on identification of reasons of low quantum efficiency and detectivity, high dark current and tend to degrade with time as well as on search of ways to overcome these deficiences. New approaches to device architecture and design as well as to principles of functioning are also desirable.
This article reports our latest data on morphology and defects of Ge/Si heterostructures. On the basis of our recent results on the photo-emf in the Si p–i–n-structures with Ge quantum dots, which are also reported in this article, we propose a new design of photovoltaic quantum dot infrared photodetectors.
Equipment and techniques
The Ge/Si samples were grown and characterized using an integrated ultrahigh vacuum instrument[9–12] built on the basis of the Riber SSC 2 surface science center with the EVA 32 molecular-beam epitaxy (MBE) chamber equipped with the RH20 reflection high-energy electron diffraction (RHEED) tool (Staib Instruments) and connected through a transfer line to the GPI-300 ultrahigh vacuum scanning tunnelling microscope (STM)[13–15]. Sources with the electron beam evaporation were used for Ge or Si deposition. A Knudsen effusion cells was utilized if boron doping was applied for QDIP p–i–n-structure formation. The pressure of about 5×10−9 Torr was kept in the preliminary sample cleaning (annealing) chamber. The MBE chamber was evacuated down to about 10−11 Torr before processes; the pressure increased to nearly 2×10−9 Torr at most during the Si substrate cleaning and 10−9 Torr during Ge or Si deposition. The residual gas pressure did not exceed 10−10 Torr in the STM chamber. Additional details of the experimental instruments and process control can be found in Ref..
RHEED measurements were carried out in situ, i.e., directly in the MBE chamber during a process. STM images were obtained in the constant tunnelling current mode at the room temperature. The STM tip was zero-biased while the sample was positively or negatively biased when scanned in empty- or filled-states imaging mode. Structural properties of the Ge/Si films were explored by using the Carl Zeiss Libra-200 FE HR HRTEM.
The images were processed using the WSxM software.
For obtaining spectra of photo-electromotive force (photo-emf) a setup enabling sample illumination by two independent beams was used; one of the beams was a wide-band infrared (IR) radiation, generated by a tungsten bulb, passed through a filter of Si or Ge (bias lighting) and the other was a beam-chopper modulated narrow-band radiation cut from globar emission by an IR monochromator tunable in the range from 0.8 to 20 μ m. The spectra were taken at the chopping frequency of 12.5 Hz at temperatures ranged from 300 to 70 K and a widely varied power of the bias lighting.
The measurements of the terahertz dynamic conductivity and absorptivity of Ge/Si heterostructures at room and cryogenic temperatures (down to 5 K) have been performed using the spectrometer based on backward-wave oscillators (BWO) as radiation sources. This advanced experimental technique will be described in detail below in a separate section.
Sample preparation procedures
Preparation of samples for STM and RHEED
Initial samples for STM and RHEED studies were 8×8 mm2 squares cut from the specially treated commercial boron-doped Czochralski-grown (CZ) Si(100) wafers (p-type, ρ=12 Ω cm). After washing and chemical treatment following the standard procedure described elsewhere, which included washing in ethanol, etching in the mixture of HNO3 and HF and rinsing in the deionized water, the silicon substrates were loaded into the airlock and transferred into the preliminary annealing chamber where they were outgassed at the temperature of around 565℃ for more than 6 h. After that, the substrates were moved for final treatment and Ge deposition into the MBE chamber where they were subjected to two-stages annealing during heating with stoppages at 600℃ for 5 min and at 800℃ for 3 min[9, 10]. The final annealing at the temperature greater than 900℃ was carried out for nearly 2.5 min with the maximum temperature of about 925℃ (1.5 min). Then, the temperature was rapidly lowered to about 750℃. The rate of the further cooling was around 0.4℃/s that corresponded to the ‘quenching’ mode applied in. The surfaces of the silicon substrates were completely purified of the oxide film as a result of this treatment[10, 18, 19].
Ge was deposited directly on the deoxidized Si(001) surface. The deposition rate was varied from about 0.1 to 0.15 Å/s; the effective Ge film thickness (hGe) was varied from 3 to 18 Å for different samples. The substrate temperature during Ge deposition (Tgr) was 360℃ for the low-temperature mode and 600 or 650℃ for the high-temperature mode. The rate of the sample cooling down to the room temperature was approximately 0.4℃/s after the deposition.
Preparation of multilayer structures
Ge/Si heterostructures with buried Ge layers were grown on CZ p-Si(100):B wafers (ρ =12 Ω cm) washed and outgassed as described above. Deoxidized Si(001) surfaces were prepared by a process allowed us to obtain clean substrate surfaces (this was verified by STM and RHEED) and perfect epitaxial interfaces with Si buffer layers (verified by HRTEM): the wafers were annealed at 800℃ under Si flux of Å/s until a total amount of the deposited Si, expressed in the units of the Si film thickness indicated by the film thickness monitor, reached 30 Å; 2-minute stoppages of Si deposition were made first twice after every 5 Å and then twice after every 10 Å.
Afterwards, a ∼ 100 nm thick Si buffer was deposited on the prepared surface at the temperature of ∼ 650℃. Then, a single Ge layer or a multilayer Ge/Si structure was grown. A number of Ge layers in multilayer structures reached 15 but usually was 5; their effective thickness (hGe), permanent for each sample, was varied from sample to sample in the range from 4 to 18 Å; the thickness of the Si spacers (hSi) was ∼ 50 nm. The Ge deposition temperature was ∼ 360℃, Si spacers were grown at ∼ 530℃. A heterostructure formed in such a way was capped by a ∼ 100 nm thick Si layer grown at ∼ 530℃. All layers were undoped.
The samples were quenched after the growth at the rate of ∼ 0.4℃/s.
Growth of p–i–n-structures
p–i–n-structures were grown on commercial phosphorus-doped CZ n-Si(100) substrates (ρ=0.1 Ω cm). Si surfaces were prepared for structure deposition in the same way as for the growth of multilayer structures. i-Si buffer domains of various thicknesses were grown on the clean surfaces at ∼ 650℃. Then, a stacked structure of several periods of quantum dot (QD) dense arrays separated by Si barriers was grown under the same conditions as the multilayer structures; hSi was widely varied in different structures reaching 50 nm; hGe always was 10 Å. A sufficiently thick undoped Si layer separated the stacked QD array from the Si:B cap doped during the growth, the both layers were grown at ∼ 530℃.
Mesas were formed on samples for photoelectric measurements. Ohmic contacts were formed by thermal deposition of aluminum.
are Fresnel coefficients for the interfaces ‘air–sample’, indices p, q=1, 2 correspond: ‘1’ to air (refractive index n1=1, extinction coefficient k1=0) and ‘2’ to the material of the sample (n2, k2),d is the sample thickness, λ is the radiation wavelength. The sample parameters (for instance, n2 and k2 ) are found for each fixed frequency by solving two coupled equations for the two unknowns, Tr(n2, k2, ν)=T rexp(ν) and φ(n2, k2, ν)=φexp(ν) [here T rexp(ν) and φexp(ν) are the measured quantities]. The so-found values of n2(ν) and k2(ν) can then be used to derive the spectra of the complex permittivity, complex conductivity, etc. ( is the high-frequency contribution to the permittivity).
If the sample is characterized by low enough absorption coefficient, Fabry–Perot-like interference of the radiation within the plane-parallel layer leads to an interference maxima and minima in the transmission coefficient spectra. In this case there is no need to measure the phase shift spectra since the pairs of optical quantities of the sample can be calculated from the transmission coefficient spectrum alone: the absorptive part (like ε′ or σ1) is determined from the interferometric maxima amplitudes and the refractive part (like ε ′ or n) is calculated from their positions[20, 21].
Main parameters of the terahertz BWO-spectrometer
Frequency range , THz
0.03 to 2
Probing radiation power, mW
1 to 100
Dynamical range, dB
40 to 60
Signal to noise ratio
104 to 106
Probing radiation polarization degree, %
Time to record a spectrum of 100 points, s:
10 to 20
20 to 40
Temperature interval, K
2 to 300
Magnetic fields, T
up to 7
Results and discussion
Morphology and defects
STM and RHEED study of Ge/Si(001) QD arrays: morphology and formation
At high temperatures (> 600℃), only pyramids represent a family of huts: they were found to nucleate on the WL patches in the same process of 16-dimer structure occurrence as at low temperatures. We failed to find wedges or their nuclei if Ge was deposited at these temperatures and this fact waits for a theoretical explanation.
In addition to pyramids, shapeless Ge heaps faceting during annealing have been observed on WL in the vicinity of pits and interpreted as possible precursors of large faceted clusters[12, 24]. Note that a mechanism of Ge hut formation via faceting of some shapeless structures appearing near WL irregularities, which resembles the process described in the current article, was previously considered as the only way of Ge cluster nucleation on Si(001)[27, 28]. Now we realize that huts nucleate in a different way and formation of the faceting heaps at high temperatures is a process competing with appearance of real pyramidal huts which arise due to formation of the 16-dimer nuclei on tops of WL patches[11, 25, 26]. Yet, further evolution of the Ge heaps into finalized faceted clusters, such as domes, in course of Ge deposition is not excluded.
RHEED has allowed as to carry our in-situ explorations of forming cluster arrays. We have compared RHEED patterns of Ge/Si(001) surfaces during Ge deposition at different temperatures and a dynamics of diffraction patterns during sample heating and cooling.
Influence of the sample annealing at the deposition temperature is illustrated by a complimentary pair of the RHEED patterns given in Figure4c,d. Annealing of specimens at the temperature of growth (650℃) resulted in appearance of the 3D-reflexes (Figure4d) that also corresponds with the results of our STM studies.
This observation reflects the process of Ge cluster “condensation” from the 2D gas of mobile Ge adatoms. High Ge mobility and low cluster nucleation rate in comparison with fluxes to competitive sinks of adatoms determines the observed difference in the surface structure formation at high temperatures as compared with that at low temperatures[12, 24] when the adatom flux to nucleating and growing clusters predominates and adatom (addimer) mobility is relatively small.
STM and HRTEM study of Ge/Si heterostructures with QD array: morphology and defects
Structures overgrown with Si were examined by means of HRTEM for structural perfection or possible defects, e.g., imperfections induced by array defects reported in Ref..
It is worth while emphasising that the stretched domains usually do not contain extended defects, as it is seen from the HRTEM micrographs, except for the cases of array defects (huge clusters) like that demonstrated in Figure7. We suppose that the extended defects in these regions arise because the strain exceeds an elastic limit near huge clusters.
Photo-emf of Ge/Si p–i–n-structures
We have investigated heteroepitaxial Si p–i–n-diodes with multilayer stacks of Ge/Si(001) QD dense arrays built in intrinsic domains and found them to exhibit the photo-emf in a wide spectral range from 0.8 to 5 μ m[32, 33]. An effect of wide-band irradiation by infrared light on the photo-emf spectra has been observed. Here we describe the most representative data obtained for two radically different structures denoted as R 163 and R 166 (Figure1).
Wavelength range from 0.8 to 1.0 μm. The photo-emf response increases with the increase in the bias lighting power, reaches maximum at P≈0.63 mW/cm2 with a Si filter and at P≈2.6 mW/cm2 with a Ge filter and decreases with further increase in the power.
Wavelength range from 1.1 to 2.6 μm. The photo-emf response decreases monotonously in this range with the increase in the power of the bias lighting with any, Si or Ge, filter.
Wavelength range > 2.6 μ m. The photo-emf response increases with the increase in the bias lighting power and comes through its maximum at P≈0.63 mW/cm2 if a Si filter is used and at P≈0.25 mW/cm2 for a Ge filter. The response decreases with further growth of the bias lighting power for a Si filter and remains unchanged when Ge filter is utilized.
Wavelength range from 0.8 to 1.0 μ m
Without bias lighting, all radiation in the Si fundamental absorption range can be believed to be absorbed in Si (cap-layer, spacers, buffer layer and substrate) and QDs are not involved in the absorption, so the total charge of QD layers remains unaltered. Electron-hole pairs are generated in the intrinsic region of the p–i–n-diode as a result of the absorption and separated by the junction field which converts the radiation to emf. However, carrier separation is hindered because of presence of the potential barriers for holes in the valence band which are produced by the charged QD layers situated in intrinsic domain. Calculated height of these barriers equals 0.1 to 0.2 eV depending on the layer position in the structure.
Transitions from QD ensemble states to the valence and conduction bands of Si start under bias lighting. Carriers excited by bias lighting do not contribute to the photo-emf signal measured at the modulation frequency of the narrow-band radiation. QDs captured a photon change their charge state. An effective layer charge decreases as a result of the absorption of the bias lighting radiation that results in reduction of potential barrier height and more efficient carrier separation in the junction field. Increase in the photo-emf response in the fundamental absorption range under bias lighting is explained by this process.
Wavelength range from 1.1 to 2.6 μ m
This band is entirely below the Si fundamental absorption range. Therefore the response in this region cannot be explained in terms of absorption in bulk Si. One can explain the presence of the photo-emf signal in this region considering the following model: Both hole transitions from the QD ensemble states to the valence band and electron transitions from the QD ensemble states to the conduction band due to absorption of photons with the energy between ∼1.12 and ∼0.4 eV are possible. The probability of every kind of the transitions is determined by the photon energy, the density of states in the QD ensemble and by effective charge of the QD layer.
It follows from theoretical studies[34, 35] and experiments on photoluminescence[36, 37] that photons with energies ranged from 0.7 to 0.9 eV are required for electron transitions from the QD states to the conduction band. However, it is necessary to mention the research of photoconductivity, in which electron transitions for low photon energy (∼0.4 eV) have been shown to be likely. The availability of these transitions is explained by dispersion of sizes and composition of QDs, effect of diffusion on the hetero-interface and deformation effects.
The likelihood of electron transitions drops rapidly with photon energy decrease because of reduction of the density of states in the QDs ensemble when approaching to the conduction band edge. This is the reason of the observed monotonous decrease in the photo-emf signal with the increase in the radiation wavelength in this range.
At the same time, bias lighting switching on leads to growth of concentration of the unmodulated (“dark”) carrier, depletion of QDs and as a consequence to the observed reduction of the photo-emf response at the chopping frequency.
Wavelength range > 2.6 μ m
As mentioned above, electron transitions can happen at low energy of the exciting radiation (∼ 0.4 eV) which correspond to wavelength of ∼ 3.1 μ m. Yet, the photo-emf signal is observed at the radiation wavelengths up to 5 μ m in our measurements. The presence of the photo-emf response in this range can only be explained if the QD layer is considered as a single ensemble of mutually interacting centers. An effective positive charge in the QD layer forms a potential well for electrons in the conduction band. This leads to reduction of energy needed for electron transitions from the QD ensemble states to the conduction band. Partial emptying of the states makes electron transitions possible and, at the same time, does not lead to significant change in the potential wells depth. As a result, electron transitions can happen at the exciting radiation energies as low as 0.25 eV. Hole transitions also can happen at these energies via a large number of excited states in the QD ensemble.
It may be concluded that the likelihood of the electron transitions decreases faster than that of the hole transitions as the exciting radiation energy decreases in the considered wavelength range. However, first it is necessary to empty the levels by the electron transitions to make possible hole transitions. This could be achieved by using an additional radiation of the spectral domain where the probability of the electron transitions is high. So, bias lighting stimulates the hole transitions by exciting electrons that leads to emptying the levels. In this case the electron concentration is not modulated as distinct from the hole concentration which is modulated at the chopper frequency. This explains the observed low magnitude of the photo-emf in the wavelength range > 2.6 μ m and its increase under bias lighting.
Influence of buffer layer thickness on photo-emf spectra
Prospective photovoltaic IR detectors
On the basis of our results on the photo-emf in the Si p–i–n-structures with Ge quantum dots, we have recently proposed a new design of photovoltaic quantum dot infrared photodetectors which enables detection of variations of photo-emf produced by the narrow-band radiation in the Si fundamental absorption range (a reference beam) under the effect of the wide-band IR radiation inducing changes in the Coulomb potential of the quantum dot ensemble which, in turn, affects the efficiency of the photovoltaic conversion of the reference beam. The quantum dot array resembles a grid of a triode in these detectors which is controlled by the detected IR light. The reference narrow-band radiation generates a potential between anode and cathode of this optically driven quantum dot triode; a magnitude of this voltage depends on the charge of the QD grid (Figure11). Such detectors can be fabricated on the basis of any appropriate semiconductor structures with potential barriers, e.g., p–i–n-structures, p n-junctions or Schottky barriers, and built-in arrays of nanostructures.
There are many ways to deliver the reference beam to the detector, e.g., by irradiating the sensor by laser or LED. We propose, however, surface plasmon polaritons delivered to the detector structures by the plasmonic waveguides[40, 41] to be applied as the reference beams in the detector circuits. This approach makes such detectors, if based on Si, fully compatible with existing CMOS fabrication processes that, in turn, opens a way to development of plasmonic IR detector arrays on the basis of the monolithic silicon technology.
THz conductivity of multilayer Ge/Si QD arrays
Here σ1 is the real part and is the imaginary part of the conductivity, is the high-frequency dielectric constant, is the DC conductivity, is the plasma frequency of the carriers condensate, n, e and m∗ are, respectively, their concentration, charge and effective mass and γ is their scattering rate. Figure14 shows the temperature variation of the plasma frequency and the scattering rate of charge carriers. Lowering of the plasma frequency is mainly connected with the carriers’ freezing out and the γ(T) behaviour is well described by a dependence, as expected.
One of the main findings of this work is that the AC conductivity and absorption coefficient of Ge/Si heterostructures have been discovered to be significantly higher than those of the structure with the same amount of germanium not organized in an array of quantum dots. Crucial role played by quantum dots is supported by a decrease of σ AC and α observed for large germanium coverage (hGe > 14 Å), when structurization into quantum dots gets less pronounced and the thickness of Ge layer becomes more uniform. On the other hand, it is worth noting that no extra absorption of terahertz radiation was detected in the samples with low coverage, hGe=4.4 and 6 Å. This can be explained either by the absence of quantum dots in that thin Ge layer or by their small sizes, by a large fraction of the free wetting layer or by relatively large distances between the clusters as compared to their sizes, i.e., by the absence or smallness of the effect of quantum dots on the dielectric properties of the heterostructure.
As seen from Figure17, the values and α≈4000 cm−1 are considerably higher than the values measured for bulk germanium, σAC(Ge)≈10−2 Ω−1cm−1, by about four orders of magnitude, and α(Ge)≈40 cm−1, by about two orders of magnitude. Assuming that the AC conductivity of heterostructure is connected with the response of (quasi) free carriers, one can express it with a standard formula σ=eμn=n e2(2πγ m∗)−1(μ is the mobility of charge carriers). Then, the observed increase has to be associated with considerable enhancement either of the mobility (suppression of scattering rate) of charge carriers within a quantum dot array or of their concentration. The second possibility has to be disregarded since the total concentration of charges in the sample (substrate plus heterostructure) remains unchanged. As far as the mobility increase is concerned, we are not aware of a mechanism that could lead to its orders of magnitude growth when charges get localized within the quantum dot array.
Another interpretation of the observed excess AC conductivity could be based on some kind of resonance absorption of terahertz radiation. Known infrared experiments exhibit resonances in quantum dot arrays that are caused by the transitions between quantized energy levels, as well as between the split levels and the continuum of the valence or conduction band[4, 44–47]. Carriers localized within quantum dots can form bound states with the carriers in the surrounding continuum (excitons) or with optical phonons (polarons), which can in turn interact with each other and form collective complexes[3, 4, 45–48]. Plasma excitations generated by electromagnetic radiation in the assembly of conducting clusters or quantum dots also have energies of about 10 meV[49–51], i.e., fall into the THz band. It is important that these effects can be observed not only at low, but at elevated temperatures as well, up to the room temperature. At this stage, we are not able to unambiguously identify the origin of the THz absorption seen at T=170 to 300 K in Ge/Si heterostructure with Ge quantum dots. Among the aforementioned, the mechanisms involving polaritons or plasma excitations seem to be least affected by thermal fluctuations and could be considered as possible candidates. To get detailed insight into microscopic nature of the observed effect, further investigations of heterostructures with various geometric and physical parameters, as well as in a wider frequency and temperature intervals are in progress.
In conclusion of the article, we highlight its main provisions.
Using high resolution STM and in-situ RHEED we have explored the processes of Ge hut cluster array formation and growth at low temperatures on the Ge/Si(001) wetting layer. Different dynamics of the RHEED patterns in the process of Ge hut array formation at low and high temperatures of Ge deposition reflects the difference in adatom mobility and their fluxes from 2D gas of mobile particles (atoms, dimers and dimer groups) on the surface which govern the nucleation rates and densities of arising Ge clusters.
HRTEM studies of multilayer Ge/Si heterostructures with buried arrays of Ge huts have shown that the domains of stretched lattice occurring over Ge clusters in Si layers at high Ge coverages usually do not contain extended defects. We suppose that the extended defects in these regions arise because the strain exceeds an elastic limit near huge clusters.
Silicon p–i–n-diodes with multilayer stacks of Ge cluster arrays built in i-domains have been found to exhibit the photo-emf in a wide spectral range from 0.8 to 5 μ m. A significant increase in photo-emf response in the fundamental absorption range under the wide-band IR radiation has been reported and explained in terms of positive and neutral charge states of the quantum dot layers and the Coulomb potential of the quantum dot ensemble. A new type of photovoltaic QDIPs is proposed in which photovoltage generated by a reference beam in the fundamental absorption band is controlled by the QD grid charge induced by the detected IR radiation.
Using a BWO-spectrometer, first measurements of terahertz dynamical conductivity spectra of Ge/Si heterostructures were carried out at frequencies ranged from 0.3 to 1.2 THz in the temperature interval from 5 to 300 K. The effective dynamical conductivity of the heterostructures with Ge quantum dots has been found to be significantly higher than that of the structure with the same amount of Ge not organized in quantum dots. The excess conductivity is not observed in the structures with the Ge coverage less than 8 Å. When a Ge/Si sample is cooled down the conductivity of the heterostructure decreases.
complementary metal-oxide semiconductor
Czochralski or grown by the Czochralski method
high resolution transmission electron microscope
light emitting diode
molecular beam epitaxy
quantum dot infrared photodetector
reflected high energy electron diffraction
secondary ion mass spectroscopy
scanning tunneling microscope
This research has been supported by the Ministry of Education and Science of RF through the contracts No. 14.740.11.0069 and 16.513.11.3046 and by RFBR through the grant No. 11-02-12023-ofi-m. Equipment of the Center of Collective Use of Scientific Equipment of GPI RAS was utilized for this study. We acknowledge the financial and technological support of this work.
We express our appreciation to Ms. Natalya Kiryanova for her valuable contribution to organization and management of this research.
- Pchelyakov OP, Bolkhovitjanov YB, Dvurechenskiĭ AV, Nikiforov AI, Yakimov AI, Voigtländer B: Molecular beam epitaxy of silicon–germanium nanostructures. Thin Solid Films 2000, 367: 75. 10.1016/S0040-6090(00)00667-2View ArticleGoogle Scholar
- Pchelyakov OP, Bolkhovitjanov YB, Sokolov LV, Nikiforov AI, Yakimov AI, Voigtländer B, Dvurechenskiĭ AV: Silicon–germanium nanostructures with quantum dots: Formation mechanisms and electrical properties. Semicond 2000, 34: 1229. 10.1134/1.1325416View ArticleGoogle Scholar
- Yakimov AI, Dvurechenskii AV, Kirienko VV, Yakovlev YI, Nikiforov AI: Long-range Coulomb interaction in arrays of self-assembled quantum dots. Phys Rev B 2000, 61: 10868. 10.1103/PhysRevB.61.10868View ArticleGoogle Scholar
- Drexler H, Leonard D, Hansen W, Kotthaus JP, Petroff PM: Spectroscopy of quantum levels in charge-tunable InGaAs quantum dots. Phys Rev Lett 1994, 73: 2252. 10.1103/PhysRevLett.73.2252View ArticleGoogle Scholar
- Lipparini E, Barberan N, Barranco M, Pi M, Serra L: Far-infrared edge modes in quantum dots. Phys Rev B 1997, 56: 12375. 10.1103/PhysRevB.56.12375View ArticleGoogle Scholar
- Wang KL, Tong S, Kim HJ: Properties and applications of SiGe nanodots. Materials Science in Semiconductor Processing 2005, 8: 389. 10.1016/j.mssp.2004.09.134View ArticleGoogle Scholar
- Wang KL, Cha D, Liu J, Chen C: Ge/Si self-assembled quantum dots and their optoelectronic device applications. Proc of the IEEE 2007, 95(9):1866.View ArticleGoogle Scholar
- Yakimov AI, Dvurechenskii AV, Nikiforov AI, Proskuryakov YY: Interlevel Ge/Si quantum dot infrared photodetector. J Appl Phys 2001, 89: 5676. 10.1063/1.1346651View ArticleGoogle Scholar
- Arapkina LV, Yuryev VA: Classification of Ge hut clusters in arrays formed by molecular beam epitaxy at low temperatures on the Si(001) surface. Phys Usp 2010, 53(3):279. [ArXiv:0907.4770] [ArXiv:0907.4770] 10.3367/UFNe.0180.201003e.0289View ArticleGoogle Scholar
- Arapkina LV, Yuryev VA, Chizh KV, Shevlyuga VM, Storojevyh MS, Krylova LA: Phase transition on the Si(001) clean surface prepared in UHV MBE chamber: A study by high resolution STM and in situ RHEED. Nanoscale Res Lett 2011, 6: 218. [ArXiv:1009.3909] [ArXiv:1009.3909] 10.1186/1556-276X-6-218View ArticleGoogle Scholar
- Arapkina LV, Yuryev VA: CMOS compatible dense arrays of Ge quantum dots on the Si(001) surface: Hut cluster nu-cleation, atomic structure, and array life cycle during UHV MBE growth. Nanoscale Res Lett 2011, 6: 345. [ArXiv:1009.3831] [ArXiv:1009.3831] 10.1186/1556-276X-6-345View ArticleGoogle Scholar
- Yuryev VA, Arapkina LV: Ge quantum dot arrays grown by ultrahigh vacuum molecular-beam epitaxy on the Si(001) surface: nucleation, morphology, and CMOS compatibility. Nanoscale Res Lett 2011, 6: 522. [ArXiv:1104.2848] [ArXiv:1104.2848] 10.1186/1556-276X-6-522View ArticleGoogle Scholar
- Eltsov KN: Ultrahigh vacuum scanning tunneling microscope STM GPI-300. [http://surface.gpi.ru/papers/gpi300e.pdf] 
- Eltsov KN, Klimov AN, Kosyakov AN, Obyedkov OV, Shevlyuga VM, Yurov VY: Ultrahigh vacuum scanning tunnelling microscope GPI-300. In Chemical state and atomic structure of fcc metal surfaces in chemical reaction with halogens, Volume 59 of Proc. of General Physics Institute. Edited by Konov VI, Eltsov KN. Moscow, Russia, Nauka; 2003:45–45.Google Scholar
- Yurov VY, Klimov AN: Scanning tunneling microscope calibration and reconstruction of real image: Drift and slope elimination. Rev Sci Instrum 1994, 65: 1551. 10.1063/1.1144890View ArticleGoogle Scholar
- Horcas I, Fernandez R, Gomez-Rodriguez JM, Colchero J, Gomez-Herrero J, Baro AM: WSxM: A software for scanning probe microscopy and a tool for nanotechnology. Rev Sci Instrum 2007, 78: 013705. 10.1063/1.2432410View ArticleGoogle Scholar
- Reinhardt KA, Kern W(Eds): Handbook of silicon wafer cleaning technology. William Andrew Inc., Norwich, NY,USA; 2008.Google Scholar
- Arapkina LV, Shevlyuga VM, Yuryev VA: Structure and peculiarities of the (8×n)-type Si(001) surface prepared in a molecular beam epitaxy chamber: A scanning tunneling microscopy study. JETP Lett 2008, 87: 215. [ArXiv:0908.1346] [ArXiv:0908.1346] 10.1134/S0021364008040085View ArticleGoogle Scholar
- Arapkina LV, Yuryev VA, Shevlyuga VM, Chizh KV: Phase transition between (2×1) and c(8×8) reconstructions observed on the Si(001) surface around 600°C. JETP Lett 2010, 92(5):310. [ArXiv:1007.0329] [ArXiv:1007.0329] 10.1134/S0021364010170091View ArticleGoogle Scholar
- Kozlov G, Volkov A: Millimeter and submillimeter wave spectroscopy of solids. In Topics in Applied Physics, Volume 74. Edited by Grüner G. Berlin Springer; 1998:51–51.Google Scholar
- Gorshunov B, Volkov A, Spektor I, Prokhorov A, Mukhin A, Dressel M, Uchida S, Loidl A: Terahertz BWO-spectroscopy. Int J Infrared Millimeter Waves 2005, 26: 1217. 10.1007/s10762-005-7600-yView ArticleGoogle Scholar
- Born M, Wolf E: Principles of Optics. Pergamon, London; 1959.Google Scholar
- Dressel M, Grüner G: Electrodynamics of Solids. Cambridge University Press, London; 2002.View ArticleGoogle Scholar
- Yuryev VA, Arapkina LV: Nucleation of Ge clusters at high temperatures on Ge/Si(001) wetting layer. J Appl Phys 2012, 111: 094307. [ArXiv:1105.6012] [ArXiv:1105.6012] 10.1063/1.4707936View ArticleGoogle Scholar
- Arapkina LV, Yuryev VA: Nucleation of Ge quantum dots on the Si(001) surface. Phys Rev B 2010, 82: 045315. [ArXiv:0907.4665] [ArXiv:0907.4665]View ArticleGoogle Scholar
- Arapkina LV, Yuryev VA: An initial phase of Ge hut array formation at low temperature on Si(001). J Appl Phys 2011, 109(10):104319. [ArXiv:1009.3831] [ArXiv:1009.3831] 10.1063/1.3592979View ArticleGoogle Scholar
- Goldfarb I, Hayden PT, Owen JHG, Briggs GAD: Nucleation of “hut” pits and clusters during gas-source molecular-beam epitaxy of Ge/Si(001) in in situ scanning tunnelling microscopy. Phys Rev Lett 1997, 78(20):3959. 10.1103/PhysRevLett.78.3959View ArticleGoogle Scholar
- Goldfarb I: Effect of strain on the appearance of subcritical nuclei of Ge nanohuts on Si(001). Phys Rev Lett 2005, 95: 025501.View ArticleGoogle Scholar
- Yuryev VA, Arapkina LV: Defects of Ge quantum dot arrays on the Si(001) surface. Physica B 2009, 404: 4719. [ArXiv:0908.0841] [ArXiv:0908.0841] 10.1016/j.physb.2009.08.118View ArticleGoogle Scholar
- Kucherenko IV, Vinogradov VS, Melnik NN, Arapkina LV, Chapnin VA, Chizh KV, Yuryev VA: Effect of interdiffusion and quantum confinement on Raman spectra of the Ge/Si(100) heterostructures with quantum dots. In Proceedings of the 16th International Symposium “Nanostructures: Physics and Technology”. Ioffe Physico-Technical Institute, St. Petersburg, Russia, Vladivostok, Russia; 2008:199–199. [ArXiv:0908.1378] [ArXiv:0908.1378]Google Scholar
- Kucherenko IV, Vinogradov VS, Mel’nik NN, Arapkina LV, Chapnin VA, Chizh KV, Yuryev VA: The role of interdiffusion and spatial confinement in the formation of resonant Raman spectra of Ge/Si(100) heterostructures with quantum-dot arrays. Phys Solid State 2008, 50: 1970. [ArXiv:1010.1927] [ArXiv:1010.1927] 10.1134/S1063783408100302View ArticleGoogle Scholar
- Arapkina LV, Storozhevykh MS, Chapnin VA, Chizh KV, Uvarov OV, Kalinushkin VP, Yuryev VA: Ge/Si(001) heterostructures with dense arrays of Ge quantum dots: Low-temperature formation, characterization by high resolution STM and TEM-, and exploration of photo-EMF spectra. In Second International Symposium on Nanotechnology, Energy and Space (“NES-2011”). Institute of Microelectronics Technology and High Purity Materials of the Russian Academy of Sciences, Chernogolovka, Moscow Region, Russia; 2011:32–32.Google Scholar
- Storozhevykh MS, Arapkina LV, Chapnin VA, Kalinushkin VP, Chizh KV, Yuryev VA: Photosensitivity of Si p–i–n-structures with Ge quantum dots and effect of IR irradiation on its magnitude. In Russian Conference and school on Actual Problems of Semiconductor Photoelectronics (“Photonics-2011”). Edited by Aseev AL, Dvurechenskiĭ AV. Novosibirsk, Russia: A. V. Rzhanov Institute of Semiconductor Physics of Siberian Brunch of the Russian Academy of Sciences; 2011:36–36.Google Scholar
- Gerasimenko NN, Parhomenko YN: Silicon as a Material for Nanoelectronics. Technosphera, Moscow, Russia; 2007.Google Scholar
- Brudnyi VN, Grinyaev SN, Dvurechenskii AV: Electronic properties of silicon with ultrasmall germanium clusters. Phys Solid State 2005, 47(11):2020. 10.1134/1.2131138View ArticleGoogle Scholar
- Talalaev VG, Cirlin GE, Tonkikh AA, Zakharov ND, Werner P, Gösele U, Tomm JW, Elsaesser T: Miniband-related 1.4–1.8 μm luminescence of Ge/Si quantum dot superlattices. Nanoscale Res Lett 2006, 1: 137. 10.1007/s11671-006-9004-xView ArticleGoogle Scholar
- Larsson M, Elfving A, Holtz PO, Hansson G, Ni WX: Photoluminescence study of Si/Ge quantum dots. Surf Sci 2003, 532–535: 832.View ArticleGoogle Scholar
- Talochkin AB, Chistokhin IB, Markov VA: Lateral photoconductivity of multilayer Ge/Si structures with Ge quantum dots. Semicond 2009, 43(8):997. 10.1134/S1063782609080077View ArticleGoogle Scholar
- Arapkina LV, Storozhevykh MS, Chizh KV, Chapnin VA: Method of detection of electromagnetic radiation and device for its implementation. Patent pending; Russian Federation Patent Application No. 2012122054 May 29, 2012.Google Scholar
- Bozhevolnyi SI, Volkov VS, Devaux E, Laluet JY, Ebbesen TW: Channel plasmon subwavelength waveguide components including interferometers and ring resonators. Nature 2006, 440: 508. 10.1038/nature04594View ArticleGoogle Scholar
- Holmgaard T, Chen Z, Bozhevolnyi SI, Markey L, Dereux A, Krasavin AV, Zayats AV: Bend- and splitting loss of dielectric-loaded surface plasmon-polariton waveguides. Optics Express 2008, 16(18):13585. 10.1364/OE.16.013585View ArticleGoogle Scholar
- Krasavin AV, Zayats AV: Silicon-based plasmonic waveguides. Optics Express 2010, 18(11):11791. 10.1364/OE.18.011791View ArticleGoogle Scholar
- Sokolov AV: Optical Properties of Metals. American Elsevier, New York; 1967.Google Scholar
- Heitmann D, Kotthaus JP: The spectroscopy of quantum dot arrays. Phys Today 1993, 46: 56.View ArticleGoogle Scholar
- Boucaud P, Thanh VL, Sauvage S, Débarre D, Bouchier D: Intraband absorption in Ge/Si self-assembled quantum dots. Appl Phys Lett 1999, 74: 401. 10.1063/1.123083View ArticleGoogle Scholar
- Weber A, Gauthier-Lafaye O, Julien FH, Brault J, Gendry M, Desieres Y, Benyattou T: Strong normal-incidence infrared absorption in self-organized InAs/InAlAs quantum dots grown on InP(001). Appl Phys Lett 1999, 74: 413. 10.1063/1.123045View ArticleGoogle Scholar
- Sauvage S, Boucaud P, Gerard JM, Thierry-Mieg V: In-plane polarized intraband absorption in InAs/GaAs self-assembled quantum dots. Phys Rev B 1998, 58: 10562. 10.1103/PhysRevB.58.10562View ArticleGoogle Scholar
- Hameau S, Isaia JN, Guldner Y, Deleporte E, Verzelen O, Ferreira R, Bastard G, Zeman J, Gerard JM: Far-infrared magnetospectroscopy of polaron states in self-assembled InAs/GaAs quantum dots. Phys Rev B 2002, 65: 085316.View ArticleGoogle Scholar
- Sikorski C, Merkt U: Spectroscopy of electronic states in InSb quantum dots. Phys Rev Lett 1989, 62: 2164. 10.1103/PhysRevLett.62.2164View ArticleGoogle Scholar
- Dahl C, Kotthaus JP, Nickel H, Schlapp W: Coulomb coupling in arrays of electron disks. Phys Rev B 1992, 46: 15590. 10.1103/PhysRevB.46.15590View ArticleGoogle Scholar
- Demel T, Heitmann D, Grambow P, Ploog K: Nonlocal dynamic response and level crossing in quantum-dot structures. Phys Rev Lett 1990, 64: 788. 10.1103/PhysRevLett.64.788View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.